Home >Documents >Concrete Mix Design School/Handouts/06 Mix...¢ Concrete Mix Design Calculations Concrete...

Date post: | 17-Feb-2020 |

Category: | ## Documents |

View: | 56 times |

Download: | 5 times |

Share this document with a friend

Transcript:

1/22/2014

1

Concrete Mix Design CalculationsCalculations

Concrete Mix Design

• Wet Cast (Slump) • Dry Cast (no Slump)• Dry Cast (no Slump)

Combination of Art and Science…

1/22/2014

2

3

Water, Cement, & Aggregate

• As the water to cement ratio increases, the strength of a concrete mix decreases.concrete mix decreases.

• As the surface area of the aggregate increases the more water will be needed to maintain a given slump.

• Coarser Surface Texture • Particle Shape • Particle Size Distribution

• As the air content increases, the strength of the concrete decreases.

4

• It’s a calculation: w/c ~ lbs. of water / lbs. of cement w/cm ~ lbs. of water / lbs. of cementitious

Water / Cementitious Ratio

Often when w/c is discussed its really w/cm that is intended as the reference

= Water cement ratio

www.concrete-pipe.org

Water cement ratio

Water needs to be drinkable or meet ASTM 1602

0.45 expressed as decimal45 lbs of water

100 lbs of cement

1/22/2014

3

5

• Specific Gravity The relative density of a material compared to water The ratio of a material’s weight to the weight of an equal

Terminology

The ratio of a material s weight to the weight of an equal volume of water

• Bulk specific gravity (SSD): Used to determine the “solid volume” (absolute volume) of a material going into concrete It is determined by submerging the material in water for y g g 24 hours in order to fill any permeable voids

6

Specific Gravity

Water: Water: Specific Specific

Gravity = 1.00Gravity = 1.00 Stone: Stone:

Specific Specific Gravity = 2.70Gravity = 2.70

yy

Same Volume, but 2.70 Times More MassSame Volume, but 2.70 Times More Mass

Cement – 3.15 Steel – 7.85

1/22/2014

4

Calculations for SSD Bulk Specific Gravity

Coarse Aggregate Using Basket Suspended in water:Coarse Aggregate Using Basket Suspended in water: B / (B B / (B -- C) = SSD Bulk Specific GravityC) = SSD Bulk Specific Gravity

where:where: B = weight of SSD sample in airB = weight of SSD sample in air C = weight of SSD sample in waterC = weight of SSD sample in water

Field Calculation of SSD Bulk Specific Gravity:Field Calculation of SSD Bulk Specific Gravity:

Weight of Aggregate @ SSDWeight of Aggregate @ SSDWeight of Aggregate @ SSDWeight of Aggregate @ SSD Weight of equal volume of water displacedWeight of equal volume of water displaced

== Specific GravitySpecific Gravity

1245 grams of SSD aggregate1245 grams of SSD aggregate ==

469.81 grams of water displaced469.81 grams of water displaced 2.652.65

8

Concrete Mix Design

It’s always about volume!

• What is absolute volume?

1/22/2014

5

9

• Relationship of Materials to Volume specific gravity of Type I Cement = 3.15

f f

What is Absolute Volume?

specific gravity of water = 1.0 1 gallon of water weights 8.33 pounds water weights 62.4 pounds / cubic foot

Pounds of Material

S.G. X 62.4 = Absolute Volume

10Basic Concrete Mix Design

Materials Pounds of material

S.G. Abs Volume

Cement 667 3.15 3.39 -

Total Cementious 667 Miller Stone 1590 2.6 9.80 Evert Sand 1242 2.65 7.51

W t 300 1 4 81Water 300 1 4.81 Air 5.5% 1.485

Total 3799 27.00 w / cm 0.45 Unit Wt. 140.72

1/22/2014

6

Basic Concrete Mix Design

Materials Pounds of material

S.G. Abs Volume

667 3.15 X 62.4

Cement 667 3.15 3.39 -

Total Cementious 667 Miller Stone 1590 2.6 9.80 Evert Sand 1242 2.65 7.51

Water 300 1 4 81

1590 2.60 X 62.4

1242 2.65 X 62.4

Water 300 1 4.81 Air 5.5% 1.485

Total 3799 27.00 w / cm 0.45 Unit Wt. 140.72

Basic Concrete Mix Design

Materials Pounds of material

S.G. Abs Volume

Cement 667 3.15 3.39 -

Total Cementious 667 Miller Stone 1590 2.6 9.80 Evert Sand 1242 2.65 7.51

Water 300 1 4 81

300 1.0 X 62.4

0.055 X 27Water 300 1 4.81 Air 5.5% 1.485

Total 3799 27.00 w / cm 0.45 Unit Wt. 140.72

0.055 X 27

1/22/2014

7

Water / Cement Ratio = W/C

Materials Pounds of material

S.G. Abs Volume

Water / Cement 300

Cement 667 3.15 3.39 -

Total Cementious 667 Miller Stone 1590 2.6 9.80 Evert Sand 1242 2.65 7.51

Water 300 1 4 81

300 667 Weight

(mass)

Water 300 1 4.81 Air 5.5% 1.485

Total 3799 27.00 w / cm 0.45 Unit Wt. 140.72

Density (unit weight)

Materials Pounds of material

S.G. Abs Volume

Design (unit weight) 3799

Cement 667 3.15 3.39 -

Total Cementious 667 Miller Stone 1590 2.6 9.80 Evert Sand 1242 2.65 7.51

Water 300 1 4 81

3799 27.0

Water 300 1 4.81 Air 5.5% 1.485

Total 3799 27.00 w / cm 0.45 Unit Wt. 140.72

@ 1.5% air, unit weight (density) = 147.26

1/22/2014

8

Mix design with Cement & Fly Ash

133 lbs. fly ash 667 Total lbs. Cm

= 20% ash

It’s about volume!

Note: lower water demand due to fly ash

- for same slump

Mix design with Cement & Fly Ash

Proportion the mix to yield 27 ft3 … but how much sand, stone …

what ratio?

Sand / Aggregate ratio is by volume

It’s about volume!

1/22/2014

9

Mix design with Cement & Fly Ash

Volume without aggregate = 8.72

27.00 - 8.72 =

18 28 ft3 required

It’s about volume!

18.28 ft required

Sand to Aggregate Ratio

Volume of Sand Volume of Total Aggregate = Rules of thumb ?

Manufactured Concrete Pipe 60-80% Packerhead Mix 45-65% Dry Cast

1/22/2014

10

Calculating sand & stone to yield 27ft3 of concrete

•Assume this concrete needs to have Sand / Aggregate ratio of 0 42•Assume this concrete needs to have Sand / Aggregate ratio of 0.42

Volume of Sand 0 42

Total Volume of Aggregate = 0.42

Volume of Sand

Volume of Sand = 7.68 ft3

18.28 ft3 = 0.42

Calculating pounds of sand

Pounds of Material = Absolute Volume

S.G. X 62.4 Absolute Volume

Pounds of Material (sand)

2.65 X 62.4 = 7.68 ft3

Evert Sand S.G. = 2.65

Sand = 1270 lbs

1/22/2014

11

Calculating pounds of stone

Pounds of Material

S G X 62 4 = Absolute Volume

S.G. X 62.4

Pounds of Material (stone)

2.60 X 62.4 = 18.28 - 7.68 = 10.60 ft3

Total Aggregate Volume

Sand Volume

Miller Stone S.G. = 2.60

Stone = 1720 lbs

SSD Mix Design

1/22/2014

12

23

Aggregate MoistureAggregate Moisture

Bone Dry or

Oven Dry

Air Dry

Saturated and

Surface Dry

Absorbed moisture

(absorption)

SSD (ideal)

Add Water

Moist Free moisture

(moisture content)

Subtract Water

Moisture Adjustments Moisture Management is Critical (How much free water)

Total aggregate moisture = aggregate absorption + free water

(TM = absorption + free water)

3.0% = 1.5% + free water, (% free water = 1.5%) 0.015 X 1720 = 26 pounds of free water on the Stone

STONE

Sand 5.5% = 0.85% + free water, (% free water = 4.65%) 0.0465 X 1270 = 59 pounds of free water on the Sand

1/22/2014

13

25

Water Adjustment If 26 + 59 pounds of water rides in on the aggregates

you must take that amount of water out of the BATCH water.

Design water

Water on aggregates

Batch water

295

-85

210

Moisture Adjustment

Total moisture = Free moisture + Aggregate absorption

SSD & batch totals will be the same

1/22/2014

14

27

28

Where can I get this?

• Portland Cement Association (PCA) 5420 Old Orchard Road Skokie, IL 60077-1083

847 966 6700 PH847 966-6700 PH 847 966-8389 FX Info @ cement.org

1/22/2014

15

29

QUESTIONS?